Multiaxial Creep-Fatigue and Creep- Ratcheting Failures of ... Reports/FY 2009/09-832 NEUP Final A...
Embed Size (px)
Transcript of Multiaxial Creep-Fatigue and Creep- Ratcheting Failures of ... Reports/FY 2009/09-832 NEUP Final A...
Multiaxial Creep-Fatigue and Creep- Ratcheting Failures of Grade 91 and
Haynes 230 Alloys Toward Addressing Design Issues of Gen IV Nuclear
Reactor Concepts Dr. Tasnim Hassan
North Carolina State University
In collaboration with: Idaho National Laboratory
Pennsylvania State University
Sue Lesica, Federal POC Richard Wright, Technical POC
Project No. 09-832
NEUP Project ID#09-832: Year 5 – 4th Quarter & Final Report Creep-Fatigue and Creep-Ratcheting Failures of Alloy 617: Experiments and Unified
Constitutive Modeling towards Addressing the ASME Code Issues
Principal Investigators: Prof. T. Hassan, North Carolina State University Prof. C.J. Lissenden, Penn State University Dr. L. Carroll, Idaho National Lab
Students: Shahriar Quayyum (PhD), Nazrul Islam (PhD), Patrick Pritchard (MS), Matthew Fenton (MS) and Yu-Chin Chan (Undergrad), NC State University.
Mainak Sengupta (MS) and Gloria Choi (MS), Penn State University
Technical Point of Contact: Dr. R. Wright, Idaho National Lab Federal Point of Contact: Dr. Susan Lesica, U.S. Department of Energy
Project Objectives: The proposed research will develop systematic sets of uniaxial and multiaxial experimental data at a very high temperature (850-950oC) for Alloy 617. The loading histories to be prescribed in the experiments will induce creep-fatigue and creep-ratcheting failure mechanisms. These experimental responses will be scrutinized in order to quantify the influences of temperature and creep on fatigue and ratcheting failures. A unified constitutive model (UCM) will be developed and validated against these experimental responses. The improved UCM will be incorporated into the widely used finite element commercial software packages ANSYS. The modified ANSYS will be validated so that it can be used for evaluating the very high temperature ASME- NH design-by-analysis methodology for Alloy 617 and thereby addressing the ASME-NH design code issues.
Year 5-4th Quarter and Final Report: This report is stating the overall, as well as, the year 5-4th quarter accomplishments.
1. Experimental Task and Outcomes: A total of 125 uniaxial and multiaxial fatigue, fatigue-creep, and ratcheting isothermal experiments for the temperature range 25-950 degree centigrade were conducted in this project. The acquired data were critically analyzed to understand the high temperature fatigue-creep- ratcheting responses of Alloy 617 and to develop an experimentally validated advanced unified constitutive model (UCM). Based on the Alloy 617 material experiment outcomes, three MS theses and seven conference papers have been published. Two journal paper manuscripts are developed (attached with this report) and will be submitted to archival journals for publications. Such a broad and systematically developed data set was not available in the past and hence will be extremely beneficial for developing ASME Design Code provisions for Alloy 617 and unified constitutive models. The data set will be extremely beneficial in designing very high temperature components, such as, intermediate heat exchanger components under thermo-mechanical fatigue loading.
2. Unified Constitutive Model Development Task and Outcomes:
A modified unified constitutive model (UCM) has been developed based on the Chaboche non- linear kinematic hardening model by incorporating advanced modeling features for simulating
uniaxial and multiaxial fatigue and ratcheting responses. Based on the knowledge learned from the experimental task, various advanced modeling features were included in the UCM. These modeling features included multiple strain range, static recovery, multiaxial ratcheting and nonpropotional cyclic hardening/softening for simulating Alloy 617 responses for a wide temperature range and loading rates. With the modified UCM it was possible to simulate the whole set of the uniaxial and multiaxial fatigue-ratcheting responses. Two PhD and one MS students dedicated their efforts in developing the robust UCM. In addition to several conference papers, one manuscript on improved UCM for uniaxial fatigue and fatigue-creep response simulations is already developed (attached with this report) for archival journal publications. The second manuscript on improved UCM for multiaxial fatigue and ratcheting response simulations is under development and will be completed by mid Nov of 2014. The recent ASME Pressure Vessels and Piping (PVP) Conference paper and results of the UCM multiaxial response simulation are presented below to demonstrate the progresses made over the last quarter. The robust UCM developed in this task was not available earlier and hence outcome of this task is a significant accomplishment of this project.
Simulation of multiaxial fatigue-ratcheting responses of Alloy 617 using the Advanced UCM: It has been demonstrated earlier that the currently available UCM in the commercial finite element software packages cannot simulate multiaxial fatigue-ratcheting responses of Alloy 617 developed under the loading histories considered in this project (see Fig. 1). Hence, multiaxial ratcheting and nonproportional cyclic hardening-softening modeling features were incorporated into the UCM (see the recent ASME PVP conference attached with this report). With the modified UCM it was possible to simulate the whole set of the multiaxial fatigue-ratcheting responses as shown in Figs. 2-4, where it is observed that the stress-strain responses, cyclic hardening/softening of equivalent stress amplitude and axial strain ratcheting responses under different temperature levels, and shear strain amplitudes and rates are simulated with very good accuracy. The nonproportional cyclic hardening responses obtained under 90-degree out of phase (MOP) loading cycles and subsequent softening under axial strain cycle for different temperature levels, strain amplitudes and rates are also simulated well as shown in Fig. 5. Detailed of the modeling can be found in the recently published article in the ASME PVP conference proceeding (included with this report).
Fig. 1. Loading histories prescribed in the multiaxial experiments Alloy 617, (a) cyclic shear strain under steady tensile stress (MR1), (b) cyclic tensile stress and shear strain along a bow-tie path (MR2), and (c) axial and shear strain cycle along a circular path (MOP, Phase II), with uniaxial strain cycles before and after phase II (Phase I and III).
Fig. 2. Experimental and simulated stress-strain responses under MR1 multiaxial loading path at 950oC, (a) shear stress-strain (equivalent) experimental response, (b) axial-shear strain (equivalent) experimental response, (c) shear stress-strain (equivalent) simulation response, (d) axial-shear strain (equivalent) simulation response.
Fig. 3. Experimental and simulated responses for MR1 load path at different temperature and shear strain rate, (a) shear stress amplitude (equivalent), (b) axial strain ratcheting rate, (c) Shear stress amplitude (equivalent), (d) axial strain ratcheting rate.
Fig. 4. Experimental and simulated responses for MR2 load path at different temperature and shear strain rate, (a) shear stress amplitude (equivalent), (b) axial strain ratcheting rate, (c) Shear stress amplitude (equivalent), (d) axial strain ratcheting rate.
Fig. 5. Experimental (Exp) and simulated (Sim) axial stress amplitude responses, demonstrating cyclic hardening/softening under uniaxial and multiaxial loading for the three phases of the MOP multiaxial loading path under different temperature levels, and shear strain amplitudes and rates.
3. Task on Incorporation of the Modified UCM into Finite Element Software ANSYS
Development of USERMATs subroutine in order to implement the modified UCM into the finite element software ANSYS has been complete during the last quarter. Such a USERMAT with advanced UCM will allow address of ASME-NH Code issues relevant to very high temperature component design using Alloy 617. Subroutines are developed for both the solid (USERMAT3D) and shell (USERMATPS) elements in ANSYS. Radial return numerical scheme is incorporated for performing the local (integration point) computations. Thus large loading increment can be prescribed for response simulations with good accuracy and efficiency. After convergence of the UCM computation at the local level, the updated variables are transferred to ANSYS for computation and iterative equilibrium check at the component or structure level. To ensure the quadratic convergence of the global Newton iteration scheme, a tangent operator was calculated based on the converged values at the material level and transferred to ANSYS. The derivation of this consistent tangent operator for both solid and shell elements, and relevant numerical issues have presented in the last quarterly report. These USERMAT subroutines in ANSYS will allow design by inelastic analysis following the procedure in ASME-NH much more accurately than was possible before.
An Experimental Study on High Temperature Uniaxial Fatigue and
Fatigue-Creep Responses of Alloy 617 P. Graham Pritchard1, Tasnim Hassan1,*, Laura Carroll2
1North Carolina State University, Raleigh, NC 2Idaho National Laboratory, Idaho Fall, ID
Next Generation Nuclear Plants